#------------------------------------------------------------------------------
#$Date: 2016-03-21 01:21:50 +0200 (Mon, 21 Mar 2016) $
#$Revision: 178377 $
#$URL: svn://www.crystallography.net/cod/cif/4/00/09/4000929.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_4000929
loop_
_publ_author_name
'Xia, Sheng-Qing'
'Bobev, Svilen'
_publ_section_title
;
 New Manganese-Bearing Antimonides and Bismuthides with Complex
 Structures. Synthesis, Structural Characterization, and Electronic
 Properties of Yb9Mn4+xPn9(Pn= Sb or Bi)†
;
_journal_issue                   3
_journal_name_full               'Chemistry of Materials'
_journal_page_first              840
_journal_paper_doi               10.1021/cm901633r
_journal_volume                  22
_journal_year                    2010
_chemical_formula_moiety         'Mn4.18 Sb9 Yb9'
_chemical_formula_sum            'Mn4.18 Sb9 Yb9'
_chemical_formula_weight         2882.76
_chemical_name_systematic
; 
 ? 
;
_space_group_IT_number           55
_symmetry_cell_setting           orthorhombic
_symmetry_space_group_name_Hall  '-P 2 2ab'
_symmetry_space_group_name_H-M   'P b a m'
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                90.00
_cell_formula_units_Z            2
_cell_length_a                   22.0140(17)
_cell_length_b                   12.2313(10)
_cell_length_c                   4.6081(4)
_cell_measurement_reflns_used    9999
_cell_measurement_temperature    90(2)
_cell_measurement_theta_max      27.1
_cell_measurement_theta_min      1.8
_cell_volume                     1240.78(18)
_computing_cell_refinement       'SMART (Bruker, 2000)'
_computing_data_collection       'SMART (Bruker, 2000)'
_computing_data_reduction        'SAINT (Bruker, 1999)'
_computing_molecular_graphics    'SHELXTL 5.1 (Sheldrick, 1994)'
_computing_publication_material  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      90(2)
_diffrn_measured_fraction_theta_full 1.000
_diffrn_measured_fraction_theta_max 1.000
_diffrn_measurement_device_type  'Bruker Smart'
_diffrn_measurement_method       ω
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0473
_diffrn_reflns_av_sigmaI/netI    0.0267
_diffrn_reflns_limit_h_max       28
_diffrn_reflns_limit_h_min       -28
_diffrn_reflns_limit_k_max       15
_diffrn_reflns_limit_k_min       -15
_diffrn_reflns_limit_l_max       5
_diffrn_reflns_limit_l_min       -5
_diffrn_reflns_number            11379
_diffrn_reflns_theta_full        27.10
_diffrn_reflns_theta_max         27.10
_diffrn_reflns_theta_min         1.85
_exptl_absorpt_coefficient_mu    45.150
_exptl_absorpt_correction_T_max  0.2653
_exptl_absorpt_correction_T_min  0.2111
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   'SADABS (Sheldrick, 2003)'
_exptl_crystal_colour            black
_exptl_crystal_density_diffrn    7.716
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       block
_exptl_crystal_F_000             2387
_exptl_crystal_size_max          0.05
_exptl_crystal_size_mid          0.05
_exptl_crystal_size_min          0.04
_refine_diff_density_max         2.758
_refine_diff_density_min         -2.205
_refine_diff_density_rms         0.364
_refine_ls_extinction_coef       0.00060(3)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   1.067
_refine_ls_matrix_type           full
_refine_ls_number_parameters     74
_refine_ls_number_reflns         1544
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.067
_refine_ls_R_factor_all          0.0299
_refine_ls_R_factor_gt           0.0241
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0185P)²+29.8751P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0525
_refine_ls_wR_factor_ref         0.0549
_reflns_number_gt                1353
_reflns_number_total             1544
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            cm901633r_si_002.cif
_cod_data_source_block           YbMnSb
_cod_depositor_comments
;
The following automatic conversions were performed:

'_symmetry_cell_setting' value 'Orthorhombic' changed to
'orthorhombic' according to
/home/saulius/struct/CIF-dictionaries/cif_core.dic dictionary named
'cif_core.dic' version 2.4.2 from 2011-04-26.

Automatic conversion script
Id: cif_fix_values 1715 2011-07-08 13:25:40Z adriana 
;
_cod_database_code               4000929
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, -y, z'
'-x+1/2, y+1/2, -z'
'x+1/2, -y+1/2, -z'
'-x, -y, -z'
'x, y, -z'
'x-1/2, -y-1/2, z'
'-x-1/2, y-1/2, z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
Yb1 Yb 0.0000 0.0000 0.5000 0.01183(18) Uani 1 4 d S
Yb2 Yb 0.13703(2) 0.13883(5) 0.0000 0.01094(14) Uani 1 2 d S
Yb3 Yb 0.09175(2) 0.44405(4) 0.0000 0.00927(14) Uani 1 2 d S
Yb4 Yb 0.26199(3) 0.38263(5) 0.0000 0.01129(14) Uani 1 2 d S
Yb5 Yb 0.39797(3) 0.21898(5) 0.5000 0.01437(15) Uani 1 2 d S
Sb1 Sb 0.0000 0.5000 0.5000 0.0084(2) Uani 1 4 d S
Sb2 Sb 0.49806(4) 0.30617(7) 0.0000 0.00993(19) Uani 1 2 d S
Sb3 Sb 0.30846(4) 0.12989(7) 0.0000 0.01149(19) Uani 1 2 d S
Sb4 Sb 0.35134(4) 0.46563(7) 0.5000 0.00843(18) Uani 1 2 d S
Sb5 Sb 0.16793(4) 0.31436(7) 0.5000 0.00796(18) Uani 1 2 d S
Mn1 Mn 0.04502(9) 0.28191(16) 0.5000 0.0094(4) Uani 1 2 d S
Mn2 Mn 0.24190(9) 0.12221(16) 0.5000 0.0112(4) Uani 1 2 d S
Mn3 Mn 0.3861(9) 0.3646(16) 0.0000 0.003(6) Uiso 0.090(9) 2 d SP
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Mn Mn 0.3368 0.7283 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Sb Sb -0.5866 1.5461 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Yb Yb -0.3850 5.5486 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
Sb4 Yb1 Sb4 180.0 7_565 3_546
Sb4 Yb1 Sb2 84.019(18) 7_565 7_566
Sb4 Yb1 Sb2 95.981(18) 3_546 7_566
Sb4 Yb1 Sb2 95.981(18) 7_565 3_545
Sb4 Yb1 Sb2 84.019(18) 3_546 3_545
Sb2 Yb1 Sb2 180.0 7_566 3_545
Sb4 Yb1 Sb2 84.019(18) 7_565 7_565
Sb4 Yb1 Sb2 95.981(18) 3_546 7_565
Sb2 Yb1 Sb2 88.36(2) 7_566 7_565
Sb2 Yb1 Sb2 91.64(2) 3_545 7_565
Sb4 Yb1 Sb2 95.981(18) 7_565 3_546
Sb4 Yb1 Sb2 84.019(18) 3_546 3_546
Sb2 Yb1 Sb2 91.64(2) 7_566 3_546
Sb2 Yb1 Sb2 88.36(2) 3_545 3_546
Sb2 Yb1 Sb2 180.0 7_565 3_546
Sb4 Yb1 Mn1 98.72(3) 7_565 .
Sb4 Yb1 Mn1 81.28(3) 3_546 .
Sb2 Yb1 Mn1 46.718(15) 7_566 .
Sb2 Yb1 Mn1 133.282(15) 3_545 .
Sb2 Yb1 Mn1 46.718(15) 7_565 .
Sb2 Yb1 Mn1 133.282(15) 3_546 .
Sb4 Yb1 Mn1 81.28(3) 7_565 5_556
Sb4 Yb1 Mn1 98.72(3) 3_546 5_556
Sb2 Yb1 Mn1 133.281(15) 7_566 5_556
Sb2 Yb1 Mn1 46.719(15) 3_545 5_556
Sb2 Yb1 Mn1 133.281(15) 7_565 5_556
Sb2 Yb1 Mn1 46.719(15) 3_546 5_556
Mn1 Yb1 Mn1 180.0 . 5_556
Sb4 Yb1 Mn3 44.6(2) 7_565 7_565
Sb4 Yb1 Mn3 135.4(2) 3_546 7_565
Sb2 Yb1 Mn3 95.8(2) 7_566 7_565
Sb2 Yb1 Mn3 84.2(2) 3_545 7_565
Sb2 Yb1 Mn3 41.7(3) 7_565 7_565
Sb2 Yb1 Mn3 138.3(3) 3_546 7_565
Mn1 Yb1 Mn3 76.3(3) . 7_565
Mn1 Yb1 Mn3 103.7(3) 5_556 7_565
Sb4 Yb1 Mn3 135.4(2) 7_565 3_546
Sb4 Yb1 Mn3 44.6(2) 3_546 3_546
Sb2 Yb1 Mn3 84.2(2) 7_566 3_546
Sb2 Yb1 Mn3 95.8(2) 3_545 3_546
Sb2 Yb1 Mn3 138.3(3) 7_565 3_546
Sb2 Yb1 Mn3 41.7(3) 3_546 3_546
Mn1 Yb1 Mn3 103.7(3) . 3_546
Mn1 Yb1 Mn3 76.3(3) 5_556 3_546
Mn3 Yb1 Mn3 180.0 7_565 3_546
Sb4 Yb1 Mn3 44.6(2) 7_565 7_566
Sb4 Yb1 Mn3 135.4(2) 3_546 7_566
Sb2 Yb1 Mn3 41.7(3) 7_566 7_566
Sb2 Yb1 Mn3 138.3(3) 3_545 7_566
Sb2 Yb1 Mn3 95.8(2) 7_565 7_566
Sb2 Yb1 Mn3 84.2(2) 3_546 7_566
Mn1 Yb1 Mn3 76.3(3) . 7_566
Mn1 Yb1 Mn3 103.7(3) 5_556 7_566
Mn3 Yb1 Mn3 75.0(3) 7_565 7_566
Mn3 Yb1 Mn3 105.0(3) 3_546 7_566
Sb4 Yb1 Mn3 135.4(2) 7_565 3_545
Sb4 Yb1 Mn3 44.6(2) 3_546 3_545
Sb2 Yb1 Mn3 138.3(3) 7_566 3_545
Sb2 Yb1 Mn3 41.7(3) 3_545 3_545
Sb2 Yb1 Mn3 84.2(2) 7_565 3_545
Sb2 Yb1 Mn3 95.8(2) 3_546 3_545
Mn1 Yb1 Mn3 103.7(3) . 3_545
Mn1 Yb1 Mn3 76.3(3) 5_556 3_545
Mn3 Yb1 Mn3 105.0(3) 7_565 3_545
Mn3 Yb1 Mn3 75.0(3) 3_546 3_545
Mn3 Yb1 Mn3 180.0 7_566 3_545
Sb2 Yb2 Sb4 102.97(2) 7_565 3_545
Sb2 Yb2 Sb4 102.97(2) 7_565 3_546
Sb4 Yb2 Sb4 94.39(3) 3_545 3_546
Sb2 Yb2 Sb5 93.62(2) 7_565 1_554
Sb4 Yb2 Sb5 84.699(17) 3_545 1_554
Sb4 Yb2 Sb5 163.13(3) 3_546 1_554
Sb2 Yb2 Sb5 93.62(2) 7_565 .
Sb4 Yb2 Sb5 163.13(3) 3_545 .
Sb4 Yb2 Sb5 84.700(17) 3_546 .
Sb5 Yb2 Sb5 91.31(3) 1_554 .
Sb2 Yb2 Mn2 134.69(3) 7_565 .
Sb4 Yb2 Mn2 114.69(4) 3_545 .
Sb4 Yb2 Mn2 51.91(4) 3_546 .
Sb5 Yb2 Mn2 113.36(4) 1_554 .
Sb5 Yb2 Mn2 52.27(4) . .
Sb2 Yb2 Mn2 134.69(2) 7_565 1_554
Sb4 Yb2 Mn2 51.92(4) 3_545 1_554
Sb4 Yb2 Mn2 114.69(4) 3_546 1_554
Sb5 Yb2 Mn2 52.27(4) 1_554 1_554
Sb5 Yb2 Mn2 113.36(4) . 1_554
Mn2 Yb2 Mn2 89.67(5) . 1_554
Sb2 Yb2 Mn3 93.8(3) 7_565 3_545
Sb4 Yb2 Mn3 49.10(8) 3_545 3_545
Sb4 Yb2 Mn3 49.10(8) 3_546 3_545
Sb5 Yb2 Mn3 133.67(5) 1_554 3_545
Sb5 Yb2 Mn3 133.67(5) . 3_545
Mn2 Yb2 Mn3 92.6(2) . 3_545
Mn2 Yb2 Mn3 92.6(2) 1_554 3_545
Sb2 Yb2 Mn1 48.20(3) 7_565 1_554
Sb4 Yb2 Mn1 84.40(3) 3_545 1_554
Sb4 Yb2 Mn1 149.28(4) 3_546 1_554
Sb5 Yb2 Mn1 47.50(3) 1_554 1_554
Sb5 Yb2 Mn1 104.92(3) . 1_554
Mn2 Yb2 Mn1 153.62(5) . 1_554
Mn2 Yb2 Mn1 88.62(4) 1_554 1_554
Mn3 Yb2 Mn1 113.8(2) 3_545 1_554
Sb2 Yb2 Mn1 48.20(3) 7_565 .
Sb4 Yb2 Mn1 149.28(4) 3_545 .
Sb4 Yb2 Mn1 84.40(3) 3_546 .
Sb5 Yb2 Mn1 104.92(3) 1_554 .
Sb5 Yb2 Mn1 47.50(3) . .
Mn2 Yb2 Mn1 88.63(4) . .
Mn2 Yb2 Mn1 153.62(5) 1_554 .
Mn3 Yb2 Mn1 113.8(2) 3_545 .
Mn1 Yb2 Mn1 81.44(4) 1_554 .
Sb2 Yb2 Sb3 169.26(3) 7_565 .
Sb4 Yb2 Sb3 84.20(2) 3_545 .
Sb4 Yb2 Sb3 84.20(2) 3_546 .
Sb5 Yb2 Sb3 78.94(2) 1_554 .
Sb5 Yb2 Sb3 78.95(2) . .
Mn2 Yb2 Sb3 44.93(2) . .
Mn2 Yb2 Sb3 44.93(2) 1_554 .
Mn3 Yb2 Sb3 97.0(3) 3_545 .
Mn1 Yb2 Sb3 125.99(3) 1_554 .
Mn1 Yb2 Sb3 125.99(3) . .
Sb2 Yb2 Yb4 137.75(2) 7_565 3_545
Sb4 Yb2 Yb4 53.318(15) 3_545 3_545
Sb4 Yb2 Yb4 53.318(15) 3_546 3_545
Sb5 Yb2 Yb4 114.917(19) 1_554 3_545
Sb5 Yb2 Yb4 114.918(19) . 3_545
Mn2 Yb2 Yb4 62.65(3) . 3_545
Mn2 Yb2 Yb4 62.65(3) 1_554 3_545
Mn3 Yb2 Yb4 44.0(3) 3_545 3_545
Mn1 Yb2 Yb4 137.39(2) 1_554 3_545
Mn1 Yb2 Yb4 137.39(2) . 3_545
Sb3 Yb2 Yb4 52.987(18) . 3_545
Sb1 Yb3 Sb1 94.428(16) 1_554 .
Sb1 Yb3 Sb3 106.878(17) 1_554 3
Sb1 Yb3 Sb3 106.878(17) . 3
Sb1 Yb3 Mn1 53.24(3) 1_554 1_554
Sb1 Yb3 Mn1 117.09(3) . 1_554
Sb3 Yb3 Mn1 131.84(3) 3 1_554
Sb1 Yb3 Mn1 117.09(3) 1_554 .
Sb1 Yb3 Mn1 53.24(3) . .
Sb3 Yb3 Mn1 131.84(3) 3 .
Mn1 Yb3 Mn1 91.77(5) 1_554 .
Sb1 Yb3 Sb5 162.80(2) 1_554 .
Sb1 Yb3 Sb5 85.317(12) . .
Sb3 Yb3 Sb5 89.57(2) 3 .
Mn1 Yb3 Sb5 111.80(4) 1_554 .
Mn1 Yb3 Sb5 49.99(4) . .
Sb1 Yb3 Sb5 85.318(12) 1_554 1_554
Sb1 Yb3 Sb5 162.80(2) . 1_554
Sb3 Yb3 Sb5 89.57(2) 3 1_554
Mn1 Yb3 Sb5 49.99(4) 1_554 1_554
Mn1 Yb3 Sb5 111.80(4) . 1_554
Sb5 Yb3 Sb5 89.89(2) . 1_554
Sb1 Yb3 Sb2 79.702(15) 1_554 7_565
Sb1 Yb3 Sb2 79.702(15) . 7_565
Sb3 Yb3 Sb2 169.95(3) 3 7_565
Mn1 Yb3 Sb2 46.25(3) 1_554 7_565
Mn1 Yb3 Sb2 46.25(3) . 7_565
Sb5 Yb3 Sb2 83.34(2) . 7_565
Sb5 Yb3 Sb2 83.34(2) 1_554 7_565
Sb1 Yb3 Yb4 132.348(8) 1_554 .
Sb1 Yb3 Yb4 132.348(8) . .
Sb3 Yb3 Yb4 57.31(2) 3 .
Mn1 Yb3 Yb4 101.12(4) 1_554 .
Mn1 Yb3 Yb4 101.12(4) . .
Sb5 Yb3 Yb4 53.148(15) . .
Sb5 Yb3 Yb4 53.147(15) 1_554 .
Sb2 Yb3 Yb4 112.64(2) 7_565 .
Sb1 Yb3 Yb2 112.120(13) 1_554 .
Sb1 Yb3 Yb2 112.120(13) . .
Sb3 Yb3 Yb2 121.03(2) 3 .
Mn1 Yb3 Yb2 59.05(3) 1_554 .
Mn1 Yb3 Yb2 59.05(3) . .
Sb5 Yb3 Yb2 52.946(15) . .
Sb5 Yb3 Yb2 52.946(15) 1_554 .
Sb2 Yb3 Yb2 48.926(18) 7_565 .
Yb4 Yb3 Yb2 63.715(14) . .
Sb1 Yb3 Yb5 105.684(16) 1_554 3_556
Sb1 Yb3 Yb5 56.080(10) . 3_556
Sb3 Yb3 Yb5 50.889(15) 3 3_556
Mn1 Yb3 Yb5 158.74(4) 1_554 3_556
Mn1 Yb3 Yb5 96.98(3) . 3_556
Sb5 Yb3 Yb5 88.477(16) . 3_556
Sb5 Yb3 Yb5 140.42(2) 1_554 3_556
Sb2 Yb3 Yb5 135.564(15) 7_565 3_556
Yb4 Yb3 Yb5 96.171(15) . 3_556
Yb2 Yb3 Yb5 141.396(11) . 3_556
Sb1 Yb3 Yb5 56.080(10) 1_554 3
Sb1 Yb3 Yb5 105.684(16) . 3
Sb3 Yb3 Yb5 50.889(15) 3 3
Mn1 Yb3 Yb5 96.98(3) 1_554 3
Mn1 Yb3 Yb5 158.74(4) . 3
Sb5 Yb3 Yb5 140.42(2) . 3
Sb5 Yb3 Yb5 88.477(16) 1_554 3
Sb2 Yb3 Yb5 135.564(15) 7_565 3
Yb4 Yb3 Yb5 96.171(15) . 3
Yb2 Yb3 Yb5 141.396(11) . 3
Yb5 Yb3 Yb5 68.716(15) 3_556 3
Mn3 Yb4 Sb4 53.98(18) . 1_554
Mn3 Yb4 Sb4 53.98(18) . .
Sb4 Yb4 Sb4 92.29(3) 1_554 .
Mn3 Yb4 Sb5 128.49(16) . 1_554
Sb4 Yb4 Sb5 87.831(16) 1_554 1_554
Sb4 Yb4 Sb5 176.29(3) . 1_554
Mn3 Yb4 Sb5 128.49(16) . .
Sb4 Yb4 Sb5 176.29(3) 1_554 .
Sb4 Yb4 Sb5 87.832(16) . .
Sb5 Yb4 Sb5 91.80(3) 1_554 .
Mn3 Yb4 Sb3 67.1(4) . .
Sb4 Yb4 Sb3 96.21(2) 1_554 .
Sb4 Yb4 Sb3 96.21(2) . .
Sb5 Yb4 Sb3 87.46(2) 1_554 .
Sb5 Yb4 Sb3 87.46(2) . .
Mn3 Yb4 Sb3 121.8(4) . 3
Sb4 Yb4 Sb3 89.90(2) 1_554 3
Sb4 Yb4 Sb3 89.90(2) . 3
Sb5 Yb4 Sb3 86.40(2) 1_554 3
Sb5 Yb4 Sb3 86.39(2) . 3
Sb3 Yb4 Sb3 171.16(2) . 3
Mn3 Yb4 Mn2 94.9(3) . 3_556
Sb4 Yb4 Mn2 102.12(3) 1_554 3_556
Sb4 Yb4 Mn2 47.06(3) . 3_556
Sb5 Yb4 Mn2 129.31(3) 1_554 3_556
Sb5 Yb4 Mn2 75.29(3) . 3_556
Sb3 Yb4 Mn2 138.88(2) . 3_556
Sb3 Yb4 Mn2 44.78(3) 3 3_556
Mn3 Yb4 Mn2 94.9(3) . 3
Sb4 Yb4 Mn2 47.06(3) 1_554 3
Sb4 Yb4 Mn2 102.12(3) . 3
Sb5 Yb4 Mn2 75.29(3) 1_554 3
Sb5 Yb4 Mn2 129.31(3) . 3
Sb3 Yb4 Mn2 138.88(2) . 3
Sb3 Yb4 Mn2 44.78(3) 3 3
Mn2 Yb4 Mn2 76.33(4) 3_556 3
Mn3 Yb4 Yb3 173.3(4) . .
Sb4 Yb4 Yb3 122.765(18) 1_554 .
Sb4 Yb4 Yb3 122.765(18) . .
Sb5 Yb4 Yb3 54.435(15) 1_554 .
Sb5 Yb4 Yb3 54.434(16) . .
Sb3 Yb4 Yb3 119.65(2) . .
Sb3 Yb4 Yb3 51.515(18) 3 .
Mn2 Yb4 Yb3 79.81(3) 3_556 .
Mn2 Yb4 Yb3 79.81(3) 3 .
Mn3 Yb4 Yb2 59.3(4) . 3
Sb4 Yb4 Yb2 52.022(15) 1_554 3
Sb4 Yb4 Yb2 52.022(15) . 3
Sb5 Yb4 Yb2 125.854(17) 1_554 3
Sb5 Yb4 Yb2 125.854(17) . 3
Sb3 Yb4 Yb2 126.33(2) . 3
Sb3 Yb4 Yb2 62.502(19) 3 3
Mn2 Yb4 Yb2 51.12(3) 3_556 3
Mn2 Yb4 Yb2 51.12(3) 3 3
Yb3 Yb4 Yb2 114.017(18) . 3
Mn3 Yb4 Yb2 128.1(4) . .
Sb4 Yb4 Yb2 130.615(15) 1_554 .
Sb4 Yb4 Yb2 130.616(15) . .
Sb5 Yb4 Yb2 51.029(15) 1_554 .
Sb5 Yb4 Yb2 51.029(15) . .
Sb3 Yb4 Yb2 61.00(2) . .
Sb3 Yb4 Yb2 110.16(2) 3 .
Mn2 Yb4 Yb2 124.20(3) 3_556 .
Mn2 Yb4 Yb2 124.20(3) 3 .
Yb3 Yb4 Yb2 58.644(14) . .
Yb2 Yb4 Yb2 172.661(19) 3 .
Mn3 Yb5 Mn3 104.0(6) . 1_556
Mn3 Yb5 Sb4 52.7(3) . .
Mn3 Yb5 Sb4 52.7(3) 1_556 .
Mn3 Yb5 Sb3 65.7(3) . .
Mn3 Yb5 Sb3 135.6(4) 1_556 .
Sb4 Yb5 Sb3 97.08(2) . .
Mn3 Yb5 Sb3 135.6(4) . 1_556
Mn3 Yb5 Sb3 65.7(3) 1_556 1_556
Sb4 Yb5 Sb3 97.08(2) . 1_556
Sb3 Yb5 Sb3 91.32(3) . 1_556
Mn3 Yb5 Mn1 95.2(4) . 7_665
Mn3 Yb5 Mn1 95.2(4) 1_556 7_665
Sb4 Yb5 Mn1 108.98(4) . 7_665
Sb3 Yb5 Mn1 127.62(2) . 7_665
Sb3 Yb5 Mn1 127.62(2) 1_556 7_665
Mn3 Yb5 Sb2 113.9(3) . 1_556
Mn3 Yb5 Sb2 47.6(4) 1_556 1_556
Sb4 Yb5 Sb2 84.88(2) . 1_556
Sb3 Yb5 Sb2 176.73(2) . 1_556
Sb3 Yb5 Sb2 91.031(16) 1_556 1_556
Mn1 Yb5 Sb2 49.13(2) 7_665 1_556
Mn3 Yb5 Sb2 47.6(4) . .
Mn3 Yb5 Sb2 113.9(3) 1_556 .
Sb4 Yb5 Sb2 84.88(2) . .
Sb3 Yb5 Sb2 91.031(16) . .
Sb3 Yb5 Sb2 176.73(2) 1_556 .
Mn1 Yb5 Sb2 49.13(2) 7_665 .
Sb2 Yb5 Sb2 86.53(2) 1_556 .
Mn3 Yb5 Sb1 121.6(3) . 3_546
Mn3 Yb5 Sb1 121.6(3) 1_556 3_546
Sb4 Yb5 Sb1 158.80(2) . 3_546
Sb3 Yb5 Sb1 97.69(2) . 3_546
Sb3 Yb5 Sb1 97.69(2) 1_556 3_546
Mn1 Yb5 Sb1 49.82(3) 7_665 3_546
Sb2 Yb5 Sb1 79.743(19) 1_556 3_546
Sb2 Yb5 Sb1 79.742(19) . 3_546
Mn3 Yb5 Mn2 96.6(4) . .
Mn3 Yb5 Mn2 96.6(4) 1_556 .
Sb4 Yb5 Mn2 90.22(4) . .
Sb3 Yb5 Mn2 46.495(14) . .
Sb3 Yb5 Mn2 46.494(14) 1_556 .
Mn1 Yb5 Mn2 160.80(5) 7_665 .
Sb2 Yb5 Mn2 136.305(13) 1_556 .
Sb2 Yb5 Mn2 136.305(13) . .
Sb1 Yb5 Mn2 110.98(3) 3_546 .
Mn3 Yb5 Yb3 93.6(3) . 3_545
Mn3 Yb5 Yb3 162.1(3) 1_556 3_545
Sb4 Yb5 Yb3 142.905(11) . 3_545
Sb3 Yb5 Yb3 49.585(18) . 3_545
Sb3 Yb5 Yb3 99.15(2) 1_556 3_545
Mn1 Yb5 Yb3 86.66(3) 7_665 3_545
Sb2 Yb5 Yb3 127.72(2) 1_556 3_545
Sb2 Yb5 Yb3 80.687(17) . 3_545
Sb1 Yb5 Yb3 48.184(10) 3_546 3_545
Mn2 Yb5 Yb3 77.54(3) . 3_545
Mn3 Yb5 Yb3 162.1(3) . 3_546
Mn3 Yb5 Yb3 93.6(3) 1_556 3_546
Sb4 Yb5 Yb3 142.905(11) . 3_546
Sb3 Yb5 Yb3 99.15(2) . 3_546
Sb3 Yb5 Yb3 49.585(18) 1_556 3_546
Mn1 Yb5 Yb3 86.66(3) 7_665 3_546
Sb2 Yb5 Yb3 80.687(17) 1_556 3_546
Sb2 Yb5 Yb3 127.72(2) . 3_546
Sb1 Yb5 Yb3 48.184(10) 3_546 3_546
Mn2 Yb5 Yb3 77.54(3) . 3_546
Yb3 Yb5 Yb3 68.716(14) 3_545 3_546
Mn1 Sb1 Mn1 180.0 5_566 .
Mn1 Sb1 Yb3 115.36(2) 5_566 .
Mn1 Sb1 Yb3 64.64(2) . .
Mn1 Sb1 Yb3 115.36(2) 5_566 1_556
Mn1 Sb1 Yb3 64.64(2) . 1_556
Yb3 Sb1 Yb3 94.427(16) . 1_556
Mn1 Sb1 Yb3 64.64(2) 5_566 5_565
Mn1 Sb1 Yb3 115.36(2) . 5_565
Yb3 Sb1 Yb3 85.573(16) . 5_565
Yb3 Sb1 Yb3 180.0 1_556 5_565
Mn1 Sb1 Yb3 64.64(2) 5_566 5_566
Mn1 Sb1 Yb3 115.36(2) . 5_566
Yb3 Sb1 Yb3 180.0 . 5_566
Yb3 Sb1 Yb3 85.573(16) 1_556 5_566
Yb3 Sb1 Yb3 94.427(16) 5_565 5_566
Mn1 Sb1 Yb5 60.37(4) 5_566 3_556
Mn1 Sb1 Yb5 119.63(4) . 3_556
Yb3 Sb1 Yb5 75.736(12) . 3_556
Yb3 Sb1 Yb5 75.736(12) 1_556 3_556
Yb3 Sb1 Yb5 104.264(12) 5_565 3_556
Yb3 Sb1 Yb5 104.264(12) 5_566 3_556
Mn1 Sb1 Yb5 119.63(4) 5_566 7_565
Mn1 Sb1 Yb5 60.37(4) . 7_565
Yb3 Sb1 Yb5 104.264(12) . 7_565
Yb3 Sb1 Yb5 104.264(12) 1_556 7_565
Yb3 Sb1 Yb5 75.736(12) 5_565 7_565
Yb3 Sb1 Yb5 75.736(12) 5_566 7_565
Yb5 Sb1 Yb5 180.0 3_556 7_565
Mn3 Sb2 Mn1 118.10(14) . 7_665
Mn3 Sb2 Mn1 118.10(14) . 7_664
Mn1 Sb2 Mn1 114.11(7) 7_665 7_664
Mn3 Sb2 Yb2 151.4(4) . 7_665
Mn1 Sb2 Yb2 73.53(4) 7_665 7_665
Mn1 Sb2 Yb2 73.53(4) 7_664 7_665
Mn3 Sb2 Yb1 79.2(3) . 3_556
Mn1 Sb2 Yb1 72.04(4) 7_665 3_556
Mn1 Sb2 Yb1 149.47(5) 7_664 3_556
Yb2 Sb2 Yb1 80.409(19) 7_665 3_556
Mn3 Sb2 Yb1 79.2(3) . 3
Mn1 Sb2 Yb1 149.47(5) 7_665 3
Mn1 Sb2 Yb1 72.04(4) 7_664 3
Yb2 Sb2 Yb1 80.409(19) 7_665 3
Yb1 Sb2 Yb1 88.36(2) 3_556 3
Mn3 Sb2 Yb5 57.2(2) . .
Mn1 Sb2 Yb5 63.07(4) 7_665 .
Mn1 Sb2 Yb5 134.22(5) 7_664 .
Yb2 Sb2 Yb5 135.095(14) 7_665 .
Yb1 Sb2 Yb5 76.015(13) 3_556 .
Yb1 Sb2 Yb5 135.53(3) 3 .
Mn3 Sb2 Yb5 57.2(2) . 1_554
Mn1 Sb2 Yb5 134.22(5) 7_665 1_554
Mn1 Sb2 Yb5 63.07(4) 7_664 1_554
Yb2 Sb2 Yb5 135.096(14) 7_665 1_554
Yb1 Sb2 Yb5 135.53(3) 3_556 1_554
Yb1 Sb2 Yb5 76.015(13) 3 1_554
Yb5 Sb2 Yb5 86.53(2) . 1_554
Mn3 Sb2 Yb3 140.2(4) . 7_665
Mn1 Sb2 Yb3 57.60(4) 7_665 7_665
Mn1 Sb2 Yb3 57.60(4) 7_664 7_665
Yb2 Sb2 Yb3 68.42(2) 7_665 7_665
Yb1 Sb2 Yb3 125.974(17) 3_556 7_665
Yb1 Sb2 Yb3 125.974(17) 3 7_665
Yb5 Sb2 Yb3 95.92(2) . 7_665
Yb5 Sb2 Yb3 95.92(2) 1_554 7_665
Mn2 Sb3 Mn2 114.98(7) 1_554 .
Mn2 Sb3 Yb3 110.37(4) 1_554 3_545
Mn2 Sb3 Yb3 110.36(4) . 3_545
Mn2 Sb3 Yb5 74.72(4) 1_554 1_554
Mn2 Sb3 Yb5 160.53(5) . 1_554
Yb3 Sb3 Yb5 79.53(2) 3_545 1_554
Mn2 Sb3 Yb5 160.53(5) 1_554 .
Mn2 Sb3 Yb5 74.72(4) . .
Yb3 Sb3 Yb5 79.53(2) 3_545 .
Yb5 Sb3 Yb5 91.32(3) 1_554 .
Mn2 Sb3 Yb4 82.19(5) 1_554 .
Mn2 Sb3 Yb4 82.19(5) . .
Yb3 Sb3 Yb4 154.29(3) 3_545 .
Yb5 Sb3 Yb4 82.59(2) 1_554 .
Yb5 Sb3 Yb4 82.59(2) . .
Mn2 Sb3 Yb4 74.02(5) 1_554 3_545
Mn2 Sb3 Yb4 74.02(5) . 3_545
Yb3 Sb3 Yb4 71.17(2) 3_545 3_545
Yb5 Sb3 Yb4 125.45(2) 1_554 3_545
Yb5 Sb3 Yb4 125.45(2) . 3_545
Yb4 Sb3 Yb4 134.54(3) . 3_545
Mn2 Sb3 Yb2 57.65(4) 1_554 .
Mn2 Sb3 Yb2 57.65(4) . .
Yb3 Sb3 Yb2 135.68(3) 3_545 .
Yb5 Sb3 Yb2 126.981(18) 1_554 .
Yb5 Sb3 Yb2 126.982(18) . .
Yb4 Sb3 Yb2 70.03(2) . .
Yb4 Sb3 Yb2 64.51(2) 3_545 .
Mn3 Sb4 Mn3 115.5(7) 1_556 .
Mn3 Sb4 Mn2 121.0(3) 1_556 3_556
Mn3 Sb4 Mn2 121.0(3) . 3_556
Mn3 Sb4 Yb2 70.3(4) 1_556 3_556
Mn3 Sb4 Yb2 154.6(4) . 3_556
Mn2 Sb4 Yb2 66.38(3) 3_556 3_556
Mn3 Sb4 Yb2 154.6(4) 1_556 3
Mn3 Sb4 Yb2 70.3(4) . 3
Mn2 Sb4 Yb2 66.38(3) 3_556 3
Yb2 Sb4 Yb2 94.39(3) 3_556 3
Mn3 Sb4 Yb5 58.7(3) 1_556 .
Mn3 Sb4 Yb5 58.7(3) . .
Mn2 Sb4 Yb5 151.81(5) 3_556 .
Yb2 Sb4 Yb5 127.763(18) 3_556 .
Yb2 Sb4 Yb5 127.763(18) 3 .
Mn3 Sb4 Yb4 129.7(4) 1_556 .
Mn3 Sb4 Yb4 54.5(4) . .
Mn2 Sb4 Yb4 76.50(3) 3_556 .
Yb2 Sb4 Yb4 142.52(3) 3_556 .
Yb2 Sb4 Yb4 74.659(15) 3 .
Yb5 Sb4 Yb4 84.12(2) . .
Mn3 Sb4 Yb4 54.5(4) 1_556 1_556
Mn3 Sb4 Yb4 129.7(4) . 1_556
Mn2 Sb4 Yb4 76.50(3) 3_556 1_556
Yb2 Sb4 Yb4 74.659(15) 3_556 1_556
Yb2 Sb4 Yb4 142.52(3) 3 1_556
Yb5 Sb4 Yb4 84.12(2) . 1_556
Yb4 Sb4 Yb4 92.29(3) . 1_556
Mn3 Sb4 Yb1 77.2(4) 1_556 3_556
Mn3 Sb4 Yb1 77.2(4) . 3_556
Mn2 Sb4 Yb1 129.66(5) 3_556 3_556
Yb2 Sb4 Yb1 80.400(19) 3_556 3_556
Yb2 Sb4 Yb1 80.400(19) 3 3_556
Yb5 Sb4 Yb1 78.53(2) . 3_556
Yb4 Sb4 Yb1 130.626(16) . 3_556
Yb4 Sb4 Yb1 130.627(15) 1_556 3_556
Mn1 Sb5 Mn2 116.37(6) . .
Mn1 Sb5 Yb4 132.557(17) . 1_556
Mn2 Sb5 Yb4 81.16(3) . 1_556
Mn1 Sb5 Yb4 132.557(17) . .
Mn2 Sb5 Yb4 81.16(3) . .
Yb4 Sb5 Yb4 91.80(3) 1_556 .
Mn1 Sb5 Yb2 72.21(3) . .
Mn2 Sb5 Yb2 64.69(3) . .
Yb4 Sb5 Yb2 145.41(3) 1_556 .
Yb4 Sb5 Yb2 78.237(14) . .
Mn1 Sb5 Yb2 72.21(3) . 1_556
Mn2 Sb5 Yb2 64.69(3) . 1_556
Yb4 Sb5 Yb2 78.237(14) 1_556 1_556
Yb4 Sb5 Yb2 145.41(3) . 1_556
Yb2 Sb5 Yb2 91.31(3) . 1_556
Mn1 Sb5 Yb3 64.01(3) . 1_556
Mn2 Sb5 Yb3 133.839(16) . 1_556
Yb4 Sb5 Yb3 72.416(16) 1_556 1_556
Yb4 Sb5 Yb3 135.44(3) . 1_556
Yb2 Sb5 Yb3 136.12(3) . 1_556
Yb2 Sb5 Yb3 73.164(15) 1_556 1_556
Mn1 Sb5 Yb3 64.01(3) . .
Mn2 Sb5 Yb3 133.839(16) . .
Yb4 Sb5 Yb3 135.44(3) 1_556 .
Yb4 Sb5 Yb3 72.418(16) . .
Yb2 Sb5 Yb3 73.163(15) . .
Yb2 Sb5 Yb3 136.12(3) 1_556 .
Yb3 Sb5 Yb3 89.89(2) 1_556 .
Sb5 Mn1 Sb2 115.44(5) . 7_565
Sb5 Mn1 Sb2 115.44(5) . 7_566
Sb2 Mn1 Sb2 114.11(7) 7_565 7_566
Sb5 Mn1 Sb1 102.04(6) . .
Sb2 Mn1 Sb1 103.69(5) 7_565 .
Sb2 Mn1 Sb1 103.69(5) 7_566 .
Sb5 Mn1 Yb3 65.99(4) . .
Sb2 Mn1 Yb3 76.16(2) 7_565 .
Sb2 Mn1 Yb3 164.94(7) 7_566 .
Sb1 Mn1 Yb3 62.12(3) . .
Sb5 Mn1 Yb3 65.99(4) . 1_556
Sb2 Mn1 Yb3 164.94(7) 7_565 1_556
Sb2 Mn1 Yb3 76.16(2) 7_566 1_556
Sb1 Mn1 Yb3 62.12(3) . 1_556
Yb3 Mn1 Yb3 91.77(5) . 1_556
Sb5 Mn1 Yb5 171.85(8) . 7_565
Sb2 Mn1 Yb5 67.80(4) 7_565 7_565
Sb2 Mn1 Yb5 67.80(4) 7_566 7_565
Sb1 Mn1 Yb5 69.81(4) . 7_565
Yb3 Mn1 Yb5 108.82(5) . 7_565
Yb3 Mn1 Yb5 108.82(5) 1_556 7_565
Sb5 Mn1 Yb2 60.30(3) . .
Sb2 Mn1 Yb2 58.27(3) 7_565 .
Sb2 Mn1 Yb2 124.68(7) 7_566 .
Sb1 Mn1 Yb2 131.62(4) . .
Yb3 Mn1 Yb2 69.76(2) . .
Yb3 Mn1 Yb2 126.21(6) 1_556 .
Yb5 Mn1 Yb2 124.88(4) 7_565 .
Sb5 Mn1 Yb2 60.29(3) . 1_556
Sb2 Mn1 Yb2 124.68(7) 7_565 1_556
Sb2 Mn1 Yb2 58.27(3) 7_566 1_556
Sb1 Mn1 Yb2 131.62(4) . 1_556
Yb3 Mn1 Yb2 126.21(6) . 1_556
Yb3 Mn1 Yb2 69.76(2) 1_556 1_556
Yb5 Mn1 Yb2 124.88(4) 7_565 1_556
Yb2 Mn1 Yb2 81.44(4) . 1_556
Sb5 Mn1 Yb1 114.38(6) . .
Sb2 Mn1 Yb1 61.24(4) 7_565 .
Sb2 Mn1 Yb1 61.24(4) 7_566 .
Sb1 Mn1 Yb1 143.58(6) . .
Yb3 Mn1 Yb1 133.03(3) . .
Yb3 Mn1 Yb1 133.03(3) 1_556 .
Yb5 Mn1 Yb1 73.77(4) 7_565 .
Yb2 Mn1 Yb1 71.47(3) . .
Yb2 Mn1 Yb1 71.47(3) 1_556 .
Sb3 Mn2 Sb3 114.98(7) 1_556 .
Sb3 Mn2 Sb4 114.56(5) 1_556 3_546
Sb3 Mn2 Sb4 114.56(5) . 3_546
Sb3 Mn2 Sb5 106.09(5) 1_556 .
Sb3 Mn2 Sb5 106.09(5) . .
Sb4 Mn2 Sb5 98.30(6) 3_546 .
Sb3 Mn2 Yb2 77.42(2) 1_556 1_556
Sb3 Mn2 Yb2 166.24(6) . 1_556
Sb4 Mn2 Yb2 61.70(4) 3_546 1_556
Sb5 Mn2 Yb2 63.04(4) . 1_556
Sb3 Mn2 Yb2 166.24(6) 1_556 .
Sb3 Mn2 Yb2 77.42(2) . .
Sb4 Mn2 Yb2 61.70(4) 3_546 .
Sb5 Mn2 Yb2 63.03(4) . .
Yb2 Mn2 Yb2 89.67(5) 1_556 .
Sb3 Mn2 Yb5 58.78(4) 1_556 .
Sb3 Mn2 Yb5 58.78(4) . .
Sb4 Mn2 Yb5 155.99(7) 3_546 .
Sb5 Mn2 Yb5 105.71(6) . .
Yb2 Mn2 Yb5 130.36(3) 1_556 .
Yb2 Mn2 Yb5 130.36(3) . .
Sb3 Mn2 Yb4 124.08(6) 1_556 3_545
Sb3 Mn2 Yb4 61.20(3) . 3_545
Sb4 Mn2 Yb4 56.43(3) 3_546 3_545
Sb5 Mn2 Yb4 129.27(4) . 3_545
Yb2 Mn2 Yb4 117.93(6) 1_556 3_545
Yb2 Mn2 Yb4 66.24(3) . 3_545
Yb5 Mn2 Yb4 106.12(4) . 3_545
Sb3 Mn2 Yb4 61.20(3) 1_556 3_546
Sb3 Mn2 Yb4 124.08(6) . 3_546
Sb4 Mn2 Yb4 56.43(3) 3_546 3_546
Sb5 Mn2 Yb4 129.27(4) . 3_546
Yb2 Mn2 Yb4 66.23(3) 1_556 3_546
Yb2 Mn2 Yb4 117.93(6) . 3_546
Yb5 Mn2 Yb4 106.12(4) . 3_546
Yb4 Mn2 Yb4 76.33(4) 3_545 3_546
Sb2 Mn3 Sb4 113.3(4) . .
Sb2 Mn3 Sb4 113.3(4) . 1_554
Sb4 Mn3 Sb4 115.5(7) . 1_554
Sb2 Mn3 Yb4 168.4(8) . .
Sb4 Mn3 Yb4 71.5(4) . .
Sb4 Mn3 Yb4 71.5(4) 1_554 .
Sb2 Mn3 Yb5 75.2(4) . 1_554
Sb4 Mn3 Yb5 165.4(7) . 1_554
Sb4 Mn3 Yb5 68.59(8) 1_554 1_554
Yb4 Mn3 Yb5 97.9(5) . 1_554
Sb2 Mn3 Yb5 75.2(4) . .
Sb4 Mn3 Yb5 68.59(8) . .
Sb4 Mn3 Yb5 165.4(7) 1_554 .
Yb4 Mn3 Yb5 97.9(5) . .
Yb5 Mn3 Yb5 104.0(6) 1_554 .
Sb2 Mn3 Yb2 114.8(6) . 3
Sb4 Mn3 Yb2 60.6(4) . 3
Sb4 Mn3 Yb2 60.6(4) 1_554 3
Yb4 Mn3 Yb2 76.8(5) . 3
Yb5 Mn3 Yb2 128.0(3) 1_554 3
Yb5 Mn3 Yb2 128.0(3) . 3
Sb2 Mn3 Yb1 59.1(3) . 3_556
Sb4 Mn3 Yb1 58.2(2) . 3_556
Sb4 Mn3 Yb1 120.2(6) 1_554 3_556
Yb4 Mn3 Yb1 128.7(4) . 3_556
Yb5 Mn3 Yb1 133.4(6) 1_554 3_556
Yb5 Mn3 Yb1 74.2(2) . 3_556
Yb2 Mn3 Yb1 70.6(3) 3 3_556
Sb2 Mn3 Yb1 59.1(3) . 3
Sb4 Mn3 Yb1 120.2(6) . 3
Sb4 Mn3 Yb1 58.2(2) 1_554 3
Yb4 Mn3 Yb1 128.7(4) . 3
Yb5 Mn3 Yb1 74.2(2) 1_554 3
Yb5 Mn3 Yb1 133.4(6) . 3
Yb2 Mn3 Yb1 70.6(3) 3 3
Yb1 Mn3 Yb1 75.0(3) 3_556 3
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
Yb1 Sb4 3.2995(8) 7_565
Yb1 Sb4 3.2995(8) 3_546
Yb1 Sb2 3.3062(7) 7_566
Yb1 Sb2 3.3062(7) 3_545
Yb1 Sb2 3.3062(7) 7_565
Yb1 Sb2 3.3062(7) 3_546
Yb1 Mn1 3.5877(19) .
Yb1 Mn1 3.5878(19) 5_556
Yb1 Mn3 3.786(15) 7_565
Yb1 Mn3 3.786(15) 3_546
Yb1 Mn3 3.786(15) 7_566
Yb1 Mn3 3.786(15) 3_545
Yb2 Sb2 3.1324(10) 7_565
Yb2 Sb4 3.1404(7) 3_545
Yb2 Sb4 3.1404(7) 3_546
Yb2 Sb5 3.2219(7) 1_554
Yb2 Sb5 3.2219(7) .
Yb2 Mn2 3.2679(14) .
Yb2 Mn2 3.2679(14) 1_554
Yb2 Mn3 3.392(19) 3_545
Yb2 Mn1 3.5318(15) 1_554
Yb2 Mn1 3.5319(15) .
Yb2 Sb3 3.7756(10) .
Yb2 Yb4 3.8421(8) 3_545
Yb3 Sb1 3.1395(4) 1_554
Yb3 Sb1 3.1395(4) .
Yb3 Sb3 3.1611(10) 3
Yb3 Mn1 3.2093(14) 1_554
Yb3 Mn1 3.2094(14) .
Yb3 Sb5 3.2615(7) .
Yb3 Sb5 3.2616(7) 1_554
Yb3 Sb2 3.6907(10) 7_565
Yb3 Yb4 3.8222(8) .
Yb3 Yb5 4.0826(7) 3_556
Yb3 Yb5 4.0826(7) 3
Yb4 Mn3 2.741(19) .
Yb4 Sb4 3.1951(7) 1_554
Yb4 Sb4 3.1951(7) .
Yb4 Sb5 3.2083(7) 1_554
Yb4 Sb5 3.2084(7) .
Yb4 Sb3 3.2563(10) .
Yb4 Sb3 3.3988(11) 3
Yb4 Mn2 3.7287(16) 3_556
Yb4 Mn2 3.7287(16) 3
Yb4 Yb2 3.8421(8) 3
Yb5 Mn3 2.924(12) .
Yb5 Mn3 2.924(12) 1_556
Yb5 Sb4 3.1867(10) .
Yb5 Sb3 3.2215(7) .
Yb5 Sb3 3.2215(7) 1_556
Yb5 Mn1 3.237(2) 7_665
Yb5 Sb2 3.3617(8) 1_556
Yb5 Sb2 3.3617(8) .
Yb5 Sb1 3.4956(6) 3_546
Yb5 Mn2 3.634(2) .
Yb5 Yb3 4.0826(7) 3_545
Yb5 Yb3 4.0826(7) 3_546
Sb1 Mn1 2.8456(19) 5_566
Sb1 Mn1 2.8456(19) .
Sb1 Yb3 3.1395(4) 1_556
Sb1 Yb3 3.1395(4) 5_565
Sb1 Yb3 3.1395(4) 5_566
Sb1 Yb5 3.4956(6) 3_556
Sb1 Yb5 3.4956(6) 7_565
Sb2 Mn3 2.566(19) .
Sb2 Mn1 2.7456(11) 7_665
Sb2 Mn1 2.7456(11) 7_664
Sb2 Yb2 3.1324(10) 7_665
Sb2 Yb1 3.3062(7) 3_556
Sb2 Yb1 3.3062(7) 3
Sb2 Yb5 3.3617(8) 1_554
Sb2 Yb3 3.6907(10) 7_665
Sb3 Mn2 2.7322(11) 1_554
Sb3 Mn2 2.7322(11) .
Sb3 Yb3 3.1610(10) 3_545
Sb3 Yb5 3.2215(7) 1_554
Sb3 Yb4 3.3988(11) 3_545
Sb4 Mn3 2.724(10) 1_556
Sb4 Mn3 2.724(10) .
Sb4 Mn2 2.807(2) 3_556
Sb4 Yb2 3.1404(7) 3_556
Sb4 Yb2 3.1404(7) 3
Sb4 Yb4 3.1951(7) 1_556
Sb4 Yb1 3.2994(8) 3_556
Sb5 Mn1 2.735(2) .
Sb5 Mn2 2.859(2) .
Sb5 Yb4 3.2084(7) 1_556
Sb5 Yb2 3.2219(7) 1_556
Sb5 Yb3 3.2615(7) 1_556
Mn1 Sb2 2.7456(11) 7_565
Mn1 Sb2 2.7456(11) 7_566
Mn1 Yb3 3.2094(14) 1_556
Mn1 Yb5 3.237(2) 7_565
Mn1 Yb2 3.5319(15) 1_556
Mn2 Sb3 2.7322(11) 1_556
Mn2 Sb4 2.807(2) 3_546
Mn2 Yb2 3.2679(14) 1_556
Mn2 Yb4 3.7287(16) 3_545
Mn2 Yb4 3.7287(16) 3_546
Mn3 Sb4 2.724(10) 1_554
Mn3 Yb5 2.924(12) 1_554
Mn3 Yb2 3.392(19) 3
Mn3 Yb1 3.786(15) 3_556
Mn3 Yb1 3.786(15) 3
